Indexing Fe-phases in/on GaN using x-ray powder diffraction
Mauro Rovezzi
1208.3420.tex
% Created 2012-08-16 Thu 16:35
\documentclass[DIV=calc,paper=a4,fontsize=11pt,captions=tableheading]{scrartcl}
\usepackage[english]{babel}% English language/hyphenation
\usepackage[babel]{csquotes}
\usepackage[T1]{fontenc}
%\usepackage[condensed,math]{kurier}
\usepackage{times}
%\usepackage[pdftex]{graphicx}
\usepackage[dvips]{graphicx}
\usepackage[a4paper,includehead,twoside,bindingoffset=2cm,scale=0.85]{geometry}
\usepackage[x11names,svgnames,table]{xcolor}
\usepackage[hang,small,labelfont=bf,up,textfont=it,up]{caption}% Custom captions under/above floats
%\usepackage{epstopdf}% Converts .eps to .pdf
%\usepackage{subfig} % Subfigures
\usepackage{longtable} %longtables
%\usepackage{booktabs}% Nicer tables
%\usepackage{fix-cm}% Custom fontsizes
%\usepackage{sectsty}% Custom sectioning (see below)
%\allsectionsfont{\usefont{OT1}{phv}{b}{n}}% bch-b-n: CharterBT-Bold font
%\sectionfont{\usefont{OT1}{phv}{b}{n}}% bch-b-n: CharterBT-Bold font
\usepackage{fancyhdr}% Needed to define custom headers/footers
\pagestyle{fancy}% Enabling the custom headers/footers
\usepackage{lastpage}
\lhead{}
\chead{}
\rhead{}
\lfoot{\footnotesize \href{mailto:mauro.rovezzi@esrf.eu}{M. Rovezzi} \textbullet ~European Synchrotron Radiation Facility, Grenoble (FR)}
\cfoot{}
\rfoot{\footnotesize Page \thepage\ of \pageref{LastPage}}% "Page 1 of 2"
\renewcommand{\headrulewidth}{0.0pt}
\renewcommand{\footrulewidth}{0.4pt}
\usepackage{paralist} %nicer to set lists more compactly
\let\itemize\compactitem
\let\description\compactdesc
\let\enumerate\compactenum
\usepackage[colorlinks=true,linkcolor=Firebrick4,urlcolor=SteelBlue4,citecolor=Firebrick4]{hyperref}
%\usepackage[style=numeric,sorting=nyt,hyperref=true,backref=true]{biblatex}
%\bibliography{/home/mauro/biblio/BIBs/library}
\renewcommand{\figurename}{Fig.}

\providecommand{\alert}[1]{\textbf{#1}}

\title{Indexing Fe-phases in/on GaN using x-ray powder diffraction}
\author{Mauro Rovezzi}
\date{October 13, 2011}
\hypersetup{
  pdfkeywords={Fe-Nitrides, MOVPE growth},
  pdfsubject={Fe-Nitrides},
  pdfcreator={Mauro Rovezzi}}

\begin{document}

\maketitle

\setcounter{tocdepth}{3}
%\tableofcontents
%\vspace*{1cm}

This document reports the x-ray powder diffraction main reflections (intensity threshold $\ge$ 100) for possible Fe-related phases forming during the metal-organic vapor phase epitaxy (MOVPE) growth of Fe in NH$_{3}$/H$_{2}$ mixture on wurtzite-GaN/sapphire. The 2$\theta$ values are given for Cu K$\alpha_{1}$ radiation (1.5406 \AA) in the range 25-100 deg (ordered by increasing 2$\theta$). The GaN(000\emph{l}) and Al$_{2}$O$_{3}$(000\emph{l}) are also reported for reference. These data are obtained from the Inorganic Crystal Structures Database (ICSD, \href{http://icsd.fiz-karlsruhe.de/}{http://icsd.fiz-karlsruhe.de/}). The access to ICSD has been provided by the European Synchrotron Radiation Facility (ESRF).

\rowcolors{2}{gray!35}{}
\begin{longtable}{|p{28mm}p{15mm}p{15mm}p{7mm}p{8mm}p{12mm}p{2mm}p{10mm}p{5mm}|}
\caption{Indexing Fe-phases in/on GaN using x-ray powder diffraction} \label{tab:Fephases}\\
\hline
 \rowcolor{gray!70} \textbf{Phase}       &  \textbf{Type}            &  \textbf{Spg.}   &  \emph{HKL}  &  2$\theta$  &  \emph{d}-sp.  &  \textbf{M.}  &  \textbf{Int.}  &  \textbf{Ref.}                \\
\hline
\endhead
\hline\multicolumn{9}{r}{Continued on next page}\
\endfoot
\endlastfoot
 $\epsilon$-Fe$_{2}$N                      &                           &  \verb~P312~     &         101  &    29.52  &        3.0238  &            6  &         1000.0  &  \cite{Jack:1952_AC}           \\
 $\epsilon$-Fe$_{3}$N                      &                           &  \verb~P312~     &         101  &    29.54  &        3.0212  &            6  &          629.3  &  \cite{Pinsker:1954_DAN}       \\
 Fe$_{24}$N$_{10}$                &                           &  \verb~P312~     &         210  &    29.59  &        3.0163  &            6  &          444.3  &  \cite{Jack:1952_AC}           \\
 Fe$_{24}$N$_{10}$                &                           &  \verb~P312~     &         120  &    29.59  &        3.0163  &            6  &          444.3  &  \cite{Jack:1952_AC}           \\
 $\epsilon$-Fe$_{3}$N                      &                           &  \verb~P312~     &         101  &    29.84  &        2.9915  &            6  &          641.1  &  \cite{Jack:1952_AC}           \\
 Fe$_{3}$O$_{4}     $                &  Al$_{2}$MgO$_{4}$          &  \verb~Fd-3mZ~   &         220  &    30.09  &        2.9678  &           12  &          284.0  &  \cite{Fleet:1981_ACB}         \\
 FeGa$_{3}$                  &  FeGa$_{3}     $      &  \verb~P42/mnm~  &         210  &    31.93  &        2.8008  &            8  &          202.7  &  \cite{Haussermann:2002_JSSC}  \\
 Fe$_{2}$O$_{3}     $                &  Al$_{2}$O$_{3}$    &  \verb~R-3c:H~   &         104  &    33.12  &        2.7028  &            6  &         1000.0  &  \cite{Blake:1966_AM}          \\
 Fe$_{24}$N$_{10}$                &  $             $        &  \verb~P312~     &         300  &    33.66  &        2.6601  &            6  &          135.5  &  \cite{Jack:1952_AC}           \\
 FeGa$_{3}        $                  &  FeGa$_{3}     $      &  \verb~P42/mnm~  &         112  &    34.00  &        2.6344  &            8  &          382.8  &  \cite{Haussermann:2002_JSSC}  \\
\hline
 \rowcolor{red!20}  GaN                  &  ZnS(2H)                  &  \verb~P63mc~    &         002  &    34.56  &        2.5931  &            2  &          360.5  &  \cite{Paszkowicz:2004_JAC}    \\
\hline
 Fe$_{3}$O$_{4}               $      &  Al$_{2}$MgO$_{4}$          &  \verb~Fd-3mZ~   &         311  &    35.44  &        2.5309  &           24  &         1000.0  &  \cite{Fleet:1981_ACB}         \\
 Fe$_{2}$O$_{3}               $      &  Al$_{2}$O$_{3}$    &  \verb~R-3c:H~   &         110  &    35.61  &        2.5190  &            6  &          732.7  &  \cite{Blake:1966_AM}          \\
 $\zeta$-Fe$_{2}$N $            $        &                           &  \verb~Pbcn~     &         021  &    37.46  &        2.3988  &            4  &          150.9  &  \cite{Hasegawa:2005_JAC}      \\
 $\epsilon$-Fe$_{3}$N $         $        &                           &  \verb~P312~     &         110  &    37.53  &        2.3945  &            6  &         1000.0  &  \cite{Pinsker:1954_DAN}       \\
 $\epsilon$-Fe$_{2}$N $         $        &                           &  \verb~P-3m1~    &         100  &    37.53  &        2.3946  &            6  &          275.5  &  \cite{Pinsker:1954_DAN}       \\
 $\epsilon$-Fe$_{2}$N $         $        &                           &  \verb~P312~     &         110  &    37.55  &        2.3935  &            6  &          497.2  &  \cite{Jack:1952_AC}           \\
 $\epsilon$-Fe$_{3}$N$_{1.39}   $      &  Mn$_{2}$N$_{1-x}$          &  \verb~P6322~    &         110  &    37.56  &        2.3928  &            6  &          156.1  &  \cite{Leineweber:2001_JAC}    \\
 $\epsilon$-Fe$_{2.3}$N $       $        &  NiAs $        $        &  \verb~P63/mmc~  &         100  &    37.64  &        2.3876  &            6  &         1000.0  &  \cite{Kim:994_JJAP}           \\
 Fe$_{3}$C                           &  Fe$_{3}$C            &  \verb~Pnma~     &         121  &    37.64  &        2.3878  &            8  &          267.9  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{3}$C$                   $        &  Fe$_{3}$C$      $      &  \verb~Pnma~     &         210  &    37.74  &        2.3818  &            4  &          244.5  &  \cite{Fruchart:1984_JSSC}     \\
 $\epsilon$-Fe$_{3}$N $         $        &  Fe$_{3}$N$_{1+x}$          &  \verb~P6322~    &         110  &    38.09  &        2.3604  &            6  &          184.5  &  \cite{Jacobs:1995_JAC}        \\
 $\epsilon$-Fe$_{3}$N $         $        &                           &  \verb~P312~     &         110  &    38.13  &        2.3580  &            6  &         1000.0  &  \cite{Jack:1952_AC}           \\
 Fe$_{24}$N$_{10}$      &                           &  \verb~P312~     &         220  &    39.07  &        2.3038  &            6  &         1000.0  &  \cite{Jack:1952_AC}           \\
 Fe$_{0.7}$Ga$_{0.3}          $      &  Mg                       &  \verb~P63/mmc~  &         100  &    39.74  &        2.2664  &            6  &          255.2  &  \cite{Schubert:1960_DN}       \\
 FeGa$_{3}                  $        &  FeGa$_{3}$               &  \verb~P42/mnm~  &         202  &    39.78  &        2.2641  &            8  &          272.3  &  \cite{Haussermann:2002_JSSC}  \\
 Fe$_{3}$C$                   $        &  Fe$_{3}$C                &  \verb~Pnma~     &         002  &    39.79  &        2.2635  &            2  &          194.2  &  \cite{Fruchart:1984_JSSC}     \\
 $\epsilon$-Fe$_{3}C          $        &  Fe$_{3}$N$_{1+x}$        &  \verb~P6322~    &         110  &    40.07  &        2.2483  &            6  &          200.9  &  \cite{Lv:2008_CMS}            \\
 Fe$_{3}$C$                   $        &  Fe$_{3}$C                &  \verb~Pnma~     &         201  &    40.62  &        2.2191  &            4  &          167.8  &  \cite{Fruchart:1984_JSSC}     \\
 FeGa$_{3}                  $        &  FeGa$_{3}$               &  \verb~P42/mnm~  &         220  &    40.71  &        2.2142  &            4  &          121.1  &  \cite{Haussermann:2002_JSSC}  \\
 $\epsilon$-Fe$_{2.3}$N $       $        &  NiAs                     &  \verb~P63/mmc~  &         002  &    40.72  &        2.2140  &            2  &          202.6  &  \cite{Kim:994_JJAP}           \\
 Fe$_{24}$N$_{10}$      &                           &  \verb~P312~     &         310  &    40.73  &        2.2134  &            6  &          170.0  &  \cite{Jack:1952_AC}           \\
 Fe$_{24}$N$_{10}$                   &                           &  \verb~P312~     &         130  &    40.73  &        2.2134  &            6  &          170.0  &  \cite{Jack:1952_AC}           \\
 $\zeta$-Fe$_{2}$N $            $        &                           &  \verb~Pbcn~     &         200  &    40.77  &        2.2115  &            2  &          310.0  &  \cite{Hasegawa:2005_JAC}      \\
 $\epsilon$-Fe$_{3}$N $         $        &  Fe$_{3}$N$_{1+x}$        &  \verb~P6322~    &         002  &    40.81  &        2.2094  &            2  &          235.2  &  \cite{Jacobs:1995_JAC}        \\
 $\epsilon$-Fe$_{3}N_{1.39}   $      &  Mn$_{2}$N$_{1-x}$        &  \verb~P6322~    &         002  &    40.82  &        2.2085  &            2  &          209.6  &  \cite{Leineweber:2001_JAC}    \\
 $\epsilon$-Fe$_{2}$N $         $        &                           &  \verb~P-3m1~    &         002  &    40.89  &        2.2050  &            2  &          373.2  &  \cite{Pinsker:1954_DAN}       \\
 $\gamma^{\prime}$-GaFe$_{3}$N            &  CaTiO$_{3}$              &  \verb~Pm-3m~    &         111  &    41.14  &        2.1924  &            8  &         1000.0  &  \cite{Houben:2009_CM}         \\
 (Ga$_{0.5}$Fe$_{0.5}$)Fe$_{3}$N    &  CaTiO$_{3}$              &  \verb~Pm-3m~    &         111  &    41.18  &        2.1905  &            8  &         1000.0  &  \cite{Houben:2009_CM}         \\
 $\gamma^{\prime}$-Fe$_{4}$N $       $      &  CaTiO$_{3}$              &  \verb~Pm-3m~    &         111  &    41.22  &        2.1882  &            8  &         1000.0  &  \cite{Jacobs:1995_JAC}        \\
\hline
 \rowcolor{blue!20} Al$_{2}$O$_{3}$      &  Al$_{2}$O$_{3}$          &  \verb~R-3c:H~   &         006  &    41.68  &        2.1650  &            2  &            1.5  &  \cite{Graham:1960_JPCS}       \\
\hline
 $\epsilon$-Fe                         &  Mg $           $       &  \verb~63/mmc~   &         100  &    42.30  &        2.1348  &            6  &          256.8  &  \cite{Clendenen:1964_JPCS}    \\
 FeGa$_{3}                    $      &  FeGa$_{3}      $     &  \verb~P42/mnm~  &         212  &    42.42  &        2.1292  &           16  &         1000.0  &  \cite{Haussermann:2002_JSSC}  \\
 Fe$_{3}$Ga $                   $      &  AuCu$_{3}      $     &  \verb~Pm-3m~    &         111  &    42.53  &        2.1241  &            8  &         1000.0  &  \cite{Suzuki:1984_MTA}        \\
 $\zeta$-Fe$_{2}$N $              $      &  $              $       &  \verb~Pbcn~     &         102  &    42.68  &        2.1166  &            4  &          500.2  &  \cite{Hasegawa:2005_JAC}      \\
 $\alpha$-Fe$_{16}$N$_{2}         $    &  $              $       &  \verb~I4/mmm~   &         202  &    42.70  &        2.1159  &            8  &         1000.0  &  \cite{Sawada:1994_PRB}        \\
 $\gamma$-Fe                           &  Cu$            $       &  \verb~Fm-3m~    &         111  &    42.83  &        2.1099  &            8  &         1000.0  &  \cite{Straumanis:1969_ZM}     \\
 $\zeta$-Fe$_{2}$N $              $      &  $              $       &  \verb~Pbcn~     &         121  &    42.85  &        2.1087  &            8  &         1000.0  &  \cite{Hasegawa:2005_JAC}      \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         211  &    42.87  &        2.1078  &            8  &          576.0  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{0.7}$Ga$_{0.3}            $    &  Mg $           $       &  \verb~P63/mmc~  &         002  &    42.89  &        2.1070  &            2  &          267.4  &  \cite{Schubert:1960_DN}       \\
 $\gamma$-FeN$_{0.0950}         $      &  $\gamma$-FeN$_{x}$         &  \verb~Fm-3m~    &         111  &    42.93  &        2.1050  &            8  &         1000.0  &  \cite{Jack:1951_PRSLA}        \\
 $\epsilon$-Fe$_{2}$N $           $      &  $              $       &  \verb~P-3m1~    &         011  &    42.94  &        2.1044  &            6  &         1000.0  &  \cite{Pinsker:1954_DAN}       \\
 $\epsilon$-Fe$_{2}$N $           $      &  $              $       &  \verb~P-3m1~    &         101  &    42.94  &        2.1044  &            6  &          819.2  &  \cite{Pinsker:1954_DAN}       \\
 $\epsilon$-Fe$_{3}$N$_{1.39}     $    &  Mn$_{2}$N$_{1-x} $   &  \verb~P6322~    &         111  &    42.95  &        2.1039  &           12  &         1000.0  &  \cite{Leineweber:2001_JAC}    \\
 $\epsilon$-Fe$_{3}$C $           $      &  Fe$_{3}$N$_{1+x} $   &  \verb~P6322~    &         002  &    43.00  &        2.1018  &            2  &          247.7  &  \cite{Lv:2008_CMS}            \\
 Fe$_{3}$O$_{4}                 $    &  Al$_{2}$MgO$_{4} $   &  \verb~Fd-3mZ~   &         400  &    43.07  &        2.0985  &            6  &          201.3  &  \cite{Fleet:1981_ACB}         \\
 Fe$_{24}$N$_{10}$                   &  $              $       &  \verb~P312~     &         102  &    43.13  &        2.0958  &            6  &          209.7  &  \cite{Jack:1952_AC}           \\
 $\alpha$-FeN$_{0.0950}         $      &  $\alpha$-FeN$_{x}$         &  \verb~I4/mmm~   &         101  &    43.15  &        2.0950  &            8  &         1000.0  &  \cite{Jack:1951_PRSLA}        \\
 $\gamma$-Fe                           &  Cu$            $       &  \verb~Fm-3m~    &         111  &    43.38  &        2.0842  &            8  &         1000.0  &  \cite{Westgren:1921_ZPC}      \\
 $\epsilon$-Fe$_{3}$N $           $      &  Fe$_{3}$N$_{1+x} $   &  \verb~P6322~    &         111  &    43.43  &        2.0820  &           12  &         1000.0  &  \cite{Jacobs:1995_JAC}        \\
 $\alpha$-Fe                           &  W $            $       &  \verb~Im-3m~    &         110  &    43.63  &        2.0729  &           12  &         1000.0  &  \cite{Basinski:1955_PRSLA}    \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         102  &    43.73  &        2.0684  &            4  &          565.9  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{0.8}$Ga$_{0.2}            $    &  W $            $       &  \verb~Im-3m~    &         110  &    44.02  &        2.0556  &           12  &         1000.0  &  \cite{Buschow:1983_JMMM}      \\
 Fe$_{3}$Ga $                   $      &  $BiF_{3}       $     &  \verb~Fm-3m~    &         220  &    44.07  &        2.0531  &           12  &         1000.0  &  \cite{Nishino:1991_SMM}       \\
 $\alpha$-Fe                           &  W $            $       &  \verb~Im-3m~    &         110  &    44.35  &        2.0407  &           12  &         1000.0  &  \cite{Swanson:1955_NBS}       \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         220  &    44.56  &        2.0315  &            4  &          526.2  &  \cite{Fruchart:1984_JSSC}     \\
 $\alpha$-Fe                           &  W $            $       &  \verb~Im-3m~    &         110  &    44.68  &        2.0267  &           12  &         1000.0  &  \cite{Straumanis:1969_ZM}     \\
 $\epsilon$-Fe                         &  Mg $           $       &  \verb~P63/mmc~  &         002  &    44.72  &        2.0250  &            2  &          285.4  &  \cite{Clendenen:1964_JPCS}    \\
 $\alpha$-Fe$_{16}$N$_{2}         $    &  $              $       &  \verb~I4/mmm~   &         220  &    44.78  &        2.0223  &            4  &          510.2  &  \cite{Sawada:1994_PRB}        \\
 $\alpha$-FeN$_{0.0950}         $      &  $\alpha$-FeN$_{x}$         &  \verb~I4/mmm~   &         110  &    44.94  &        2.0153  &            4  &          473.3  &  \cite{Jack:1951_PRSLA}        \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         031  &    45.00  &        2.0127  &            4  &         1000.0  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{0.7}$Ga$_{0.3}            $    &  Mg $           $       &  \verb~P63/mmc~  &         101  &    45.40  &        1.9960  &           12  &         1000.0  &  \cite{Schubert:1960_DN}       \\
 $\epsilon$-Fe$_{3}$C $           $      &  Fe$_{3}$N$_{1+x} $   &  \verb~P6322~    &         111  &    45.73  &        1.9825  &           12  &         1000.0  &  \cite{Lv:2008_CMS}            \\
 $\gamma$-Fe                           &  Cu$            $       &  \verb~Fm-3m~    &         111  &    45.78  &        1.9803  &            8  &         1000.0  &  \cite{Haglund:1993_PRB}       \\
 FeGa$_{3}                    $      &  FeGa$_{3}      $     &  \verb~P42/mnm~  &         310  &    45.78  &        1.9805  &            8  &          561.4  &  \cite{Haussermann:2002_JSSC}  \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         112  &    45.85  &        1.9774  &            8  &          487.1  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{24}$N$_{10}$                   &  $              $       &  \verb~P312~     &         112  &    46.17  &        1.9646  &            6  &          199.8  &  \cite{Jack:1952_AC}           \\
 Fe$_{24}$N$_{10}$                   &  $              $       &  \verb~P312~     &        11$\bar{2}$  &    46.17  &        1.9646  &            6  &          199.8  &  \cite{Jack:1952_AC}           \\
 $\epsilon$-Fe$_{3}$N $           $      &  $              $       &  \verb~P312~     &         012  &    46.92  &        1.9348  &            6  &          168.8  &  \cite{Jack:1952_AC}           \\
 $\gamma^{\prime}$-GaFe$_{3}$N            &  CaTiO$_{3}     $     &  \verb~Pm-3m~    &         200  &    47.87  &        1.8987  &            6  &          557.0  &  \cite{Houben:2009_CM}         \\
 (Ga$_{0.5}$Fe$_{0.5}$)Fe$_{3}$N     &  CaTiO$_{3}     $     &  \verb~Pm-3m~    &         200  &    47.91  &        1.8971  &            6  &          558.2  &  \cite{Houben:2009_CM}         \\
 $\gamma^{\prime}$-Fe$_{4}$N $         $    &  CaTiO$_{3}     $     &  \verb~Pm-3m~    &         200  &    47.97  &        1.8950  &            6  &          569.3  &  \cite{Jacobs:1995_JAC}        \\
 $\epsilon$-Fe                         &  Mg $           $       &  \verb~P63/mmc~  &         101  &    48.18  &        1.8885  &           12  &         1000.0  &  \cite{Clendenen:1964_JPCS}    \\
 $\epsilon$-Fe$_{2}$N $           $      &  $              $       &  \verb~P312~     &         021  &    48.47  &        1.8767  &            6  &          215.5  &  \cite{Jack:1952_AC}           \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         131  &    48.60  &        1.8718  &            8  &          332.7  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         221  &    49.11  &        1.8535  &            8  &          409.1  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{2}$O$_{3}                 $    &  Al$_{2}$O$_{3}$   &  \verb~R-3c:H~   &         024  &    49.42  &        1.8428  &            6  &          359.4  &  \cite{Blake:1966_AM}          \\
 Fe$_{3}$Ga $                   $      &  AuCu$_{3}      $     &  \verb~Pm-3m~    &         200  &    49.51  &        1.8395  &            6  &          452.6  &  \cite{Suzuki:1984_MTA}        \\
 $\epsilon$-Fe$_{3}$N $           $      &  $              $       &  \verb~P312~     &         021  &    49.16  &        1.8519  &            6  &          145.1  &  \cite{Jack:1952_AC}           \\
 $\gamma$-Fe                           &  Cu$            $       &  \verb~Fm-3m~    &         200  &    49.87  &        1.8272  &            6  &          448.5  &  \cite{Straumanis:1969_ZM}     \\
 $\gamma$-FeN$_{0.0950}         $      &  $\gamma$-FeN$_{x}$         &  \verb~Fm-3m~    &         200  &    49.99  &        1.8230  &            6  &          484.7  &  \cite{Jack:1951_PRSLA}        \\
 $\gamma$-Fe                           &  Cu$            $       &  \verb~Fm-3m~    &         200  &    50.52  &        1.8050  &            6  &          446.7  &  \cite{Westgren:1921_ZPC}      \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         122  &    51.82  &        1.7629  &            8  &          170.7  &  \cite{Fruchart:1984_JSSC}     \\
 $\gamma$-Fe                           &  Cu$            $       &  \verb~Fm-3m~    &         200  &    53.38  &        1.7150  &            6  &          439.3  &  \cite{Haglund:1993_PRB}       \\
 Fe$_{2}$O$_{3}                 $    &  Al$_{2}$O$_{3}$      &  \verb~R-3c:H~   &         116  &    54.00  &        1.6966  &            6  &          213.7  &  \cite{Blake:1966_AM}          \\
 Fe$_{2}$O$_{3}                 $    &  Al$_{2}$O$_{3}$      &  \verb~R-3c:H~   &        11$\bar{6}$  &    54.00  &        1.6966  &            6  &          213.7  &  \cite{Blake:1966_AM}          \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         230  &    54.42  &        1.6847  &            4  &          116.1  &  \cite{Fruchart:1984_JSSC}     \\
 $\gamma$-Fe                           &  Cu$            $       &  \verb~Fm-3m~    &         111  &    55.60  &        1.6517  &            8  &         1000.0  &  \cite{Owen:1921_PM}           \\
 FeGa$_{3}                    $      &  FeGa$_{3}      $     &  \verb~P42/mnm~  &         004  &    56.08  &        1.6386  &            2  &          160.8  &  \cite{Haussermann:2002_JSSC}  \\
 $\zeta$-Fe$_{2}$N $              $      &  $              $       &  \verb~bcn~      &         221  &    56.55  &        1.6260  &            8  &          176.6  &  \cite{Hasegawa:2005_JAC}      \\
 $\epsilon$-Fe$_{2.3}$N $         $      &  NiAs $         $       &  \verb~P63/mmc~  &         102  &    56.65  &        1.6235  &           12  &          764.3  &  \cite{Kim:994_JJAP}           \\
 $\epsilon$-Fe$_{3}N_{1.39}     $    &  Mn$_{2}$N$_{1-x} $   &  \verb~P6322~    &         112  &    56.67  &        1.6229  &           12  &          189.7  &  \cite{Leineweber:2001_JAC}    \\
 Fe$_{3}$O$_{4}                 $    &  Al$_{2}$MgO$_{4} $   &  \verb~Fd-3mZ~   &         511  &    56.96  &        1.6154  &           24  &          235.6  &  \cite{Fleet:1981_ACB}         \\
 $\epsilon$-Fe$_{3}$N $           $      &  Fe$_{3}$N$_{1+x} $   &  \verb~P6322~    &         112  &    57.05  &        1.6130  &           12  &          166.7  &  \cite{Jacobs:1995_JAC}        \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         301  &    57.98  &        1.5893  &            4  &          151.0  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{0.7}$Ga$_{0.3}$                &  Mg $           $       &  \verb~P63/mmc~  &         102  &    59.89  &        1.5431  &           12  &          126.5  &  \cite{Schubert:1960_DN}       \\
 $\epsilon$-Fe$_{3}$C $           $      &  Fe$_{3}$N$_{1+x} $   &  \verb~P6322~    &         112  &    60.22  &        1.5354  &           12  &          150.1  &  \cite{Lv:2008_CMS}            \\
 Fe$_{2}$O$_{3}                 $    &  Al$_{2}$O$_{3}$      &  \verb~R-3c:H~   &        12$\bar{4}$  &    62.38  &        1.4873  &            6  &          141.2  &  \cite{Blake:1966_AM}          \\
 Fe$_{2}$O$_{3}                 $    &  Al$_{2}$O$_{3}$      &  \verb~R-3c:H~   &         214  &    62.38  &        1.4873  &            6  &          141.2  &  \cite{Blake:1966_AM}          \\
 Fe$_{3}$O$_{4}                 $    &  Al$_{2}$MgO$_{4} $   &  \verb~Fd-3mZ~   &         440  &    62.54  &        1.4839  &           12  &          388.9  &  \cite{Fleet:1981_ACB}         \\
 $\epsilon$-Fe                         &  Mg $           $       &  \verb~P63/mmc~  &         102  &    63.24  &        1.4692  &           12  &          123.7  &  \cite{Clendenen:1964_JPCS}    \\
 $\alpha$-Fe                           &  W $            $       &  \verb~Im-3m~    &         200  &    63.41  &        1.4657  &            6  &          131.9  &  \cite{Basinski:1955_PRSLA}    \\
 Fe$_{2}$O$_{3}                 $    &  Al$_{2}$O$_{3}$      &  \verb~R-3c:H~   &         300  &    63.96  &        1.4543  &            6  &          270.2  &  \cite{Blake:1966_AM}          \\
 Fe$_{0.8}$Ga$_{0.2}            $    &  W $            $       &  \verb~Im-3m~    &         200  &    64.00  &        1.4535  &            6  &          133.1  &  \cite{Buschow:1983_JMMM}      \\
 Fe$_{3}$Ga $                   $      &  $BiF_{3}       $     &  \verb~Fm-3m~    &         400  &    64.09  &        1.4518  &            6  &          133.5  &  \cite{Nishino:1991_SMM}       \\
 $\alpha$-Fe                           &  W $            $       &  \verb~Im-3m~    &         200  &    64.53  &        1.4430  &            6  &          130.3  &  \cite{Swanson:1955_NBS}       \\
 $\alpha$-Fe                           &  W $            $       &  \verb~Im-3m~    &         200  &    65.03  &        1.4331  &            6  &          129.7  &  \cite{Straumanis:1969_ZM}     \\
 $\gamma$-Fe                           &  Cu$            $       &  \verb~Fm-3m~    &         200  &    65.16  &        1.4304  &            6  &          414.5  &  \cite{Owen:1921_PM}           \\
 $\alpha$-Fe$_{16}$N$_{2}         $    &  $              $       &  \verb~I4/mmm~   &         400  &    65.18  &        1.4300  &            4  &          130.2  &  \cite{Sawada:1994_PRB}        \\
 $\alpha$-FeN$_{0.0950}         $      &  $\alpha$-FeN$_{x}$         &  \verb~I4/mmm~   &         200  &    65.44  &        1.4250  &            4  &          121.6  &  \cite{Jack:1951_PRSLA}        \\
 $\zeta$-Fe$_{2}$N $              $      &  $              $       &  \verb~Pbcn~     &         023  &    67.34  &        1.3894  &            4  &          155.8  &  \cite{Hasegawa:2005_JAC}      \\
 $\epsilon$-Fe$_{2}$N $           $      &  $              $       &  \verb~P-3m1~    &         110  &    67.72  &        1.3825  &            6  &          309.9  &  \cite{Pinsker:1954_DAN}       \\
 $\epsilon$-Fe$_{3}$N $           $      &  $              $       &  \verb~P312~     &         300  &    67.72  &        1.3825  &            6  &          287.6  &  \cite{Pinsker:1954_DAN}       \\
 $\epsilon$-Fe$_{2}$N $           $      &  $              $       &  \verb~P312~     &         300  &    67.75  &        1.3819  &            6  &          175.9  &  \cite{Jack:1952_AC}           \\
 $\epsilon$-Fe$_{3}N_{1.39}     $    &  Mn$_{2}$N$_{1-x} $   &  \verb~P6322~    &         300  &    67.78  &        1.3815  &            6  &          176.6  &  \cite{Leineweber:2001_JAC}    \\
 $\epsilon$-Fe$_{2.3}$N $         $      &  NiAs $         $       &  \verb~P63/mmc~  &         110  &    67.94  &        1.3785  &            6  &          223.8  &  \cite{Kim:994_JJAP}           \\
 FeGa$_{3}                    $      &  FeGa$_{3}      $     &  \verb~P42/mnm~  &         412  &    67.96  &        1.3781  &           16  &          130.0  &  \cite{Haussermann:2002_JSSC}  \\
 $\epsilon$-Fe$_{3}$N $           $      &  Fe$_{3}$N$_{1+x} $   &  \verb~P6322~    &         300  &    68.83  &        1.3628  &            6  &          154.6  &  \cite{Jacobs:1995_JAC}        \\
 $\epsilon$-Fe$_{3}$N $           $      &  $              $       &  \verb~P312~     &         300  &    68.92  &        1.3614  &            6  &          282.8  &  \cite{Jack:1952_AC}           \\
 FeGa$_{3}                    $      &  FeGa$_{3}      $     &  \verb~P42/mnm~  &         332  &    69.82  &        1.3459  &            8  &          110.1  &  \cite{Haussermann:2002_JSSC}  \\
 $\gamma^{\prime}$-GaFe$_{3}$N            &  CaTiO$_{3}     $     &  \verb~Pm-3m~    &         220  &    70.02  &        1.3426  &           12  &          277.6  &  \cite{Houben:2009_CM}         \\
 (Ga$_{0.5}$Fe$_{0.5}$)Fe$_{3}$N     &  CaTiO$_{3}     $     &  \verb~Pm-3m~    &         220  &    70.09  &        1.3414  &           12  &          275.8  &  \cite{Houben:2009_CM}         \\
 $\gamma^{\prime}$-Fe$_{4}$N $         $    &  CaTiO$_{3}     $     &  \verb~Pm-3m~    &         220  &    70.18  &        1.3400  &           12  &          295.8  &  \cite{Jacobs:1995_JAC}        \\
 Fe$_{24}$N$_{10}$                   &  $              $       &  \verb~P312~     &         600  &    70.78  &        1.3301  &            6  &          297.9  &  \cite{Jack:1952_AC}           \\
 Fe$_{3}$C$                     $      &  Fe$_{3}$C$       $     &  \verb~Pnma~     &         123  &    70.81  &        1.3295  &            8  &          153.0  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{0.7}$Ga$_{0.3}$                &  Mg $           $       &  \verb~P63/mmc~  &         110  &    72.13  &        1.3085  &            6  &          127.2  &  \cite{Schubert:1960_DN}       \\
 Fe$_{3}$Ga $                   $      &  AuCu$_{3}      $     &  \verb~Pm-3m~    &         220  &    72.63  &        1.3007  &           12  &          224.5  &  \cite{Suzuki:1984_MTA}        \\
 $\epsilon$-Fe$_{3}$C $           $      &  Fe$_{3}$N$_{1+x} $   &  \verb~P6322~    &         300  &    72.80  &        1.2980  &            6  &          129.7  &  \cite{Lv:2008_CMS}            \\
\hline
 \rowcolor{red!20}  GaN                  &  ZnS(2H)                  &  \verb~P63mc~    &         004  &    72.90  &        1.2965  &            2  &           25.9  &  \cite{Paszkowicz:2004_JAC}    \\
\hline
 $\gamma$-Fe                           &  Cu$             $      &  \verb~Fm-3m~    &         220  &    73.19  &        1.2920  &           12  &          217.1  &  \cite{Straumanis:1969_ZM}     \\
 $\gamma$-FeN$_{0.0950}        $       &  $\gamma$-FeN$_{x} $    &  \verb~Fm-3m~    &         220  &    73.39  &        1.2891  &           12  &          233.3  &  \cite{Jack:1951_PRSLA}        \\
 $\gamma$-Fe                           &  Cu$             $      &  \verb~Fm-3m~    &         220  &    74.24  &        1.2763  &           12  &          214.9  &  \cite{Westgren:1921_ZPC}      \\
 FeGa$_{3}                   $       &  FeGa$_{3}       $    &  \verb~P42/mnm~  &         314  &    75.20  &        1.2625  &           16  &          227.9  &  \cite{Haussermann:2002_JSSC}  \\
 $\zeta$-Fe$_{2}$N $             $       &  $               $      &  \verb~Pbcn~     &         321  &    75.65  &        1.2561  &            8  &          128.5  &  \cite{Hasegawa:2005_JAC}      \\
 $\epsilon$-Fe$_{3}N_{1.39}    $     &  Mn$_{2}$N$_{1-x}  $  &  \verb~P6322~    &         113  &    75.80  &        1.2540  &           12  &          157.7  &  \cite{Leineweber:2001_JAC}    \\
 $\epsilon$-Fe$_{3}$N $          $       &  Fe$_{3}$N$_{1+x}  $  &  \verb~P6322~    &         113  &    76.11  &        1.2496  &           12  &          151.7  &  \cite{Jacobs:1995_JAC}        \\
 $\epsilon$-Fe$_{3}$N $          $       &  $               $      &  \verb~P312~     &         113  &    76.50  &        1.2442  &            6  &          140.7  &  \cite{Jack:1952_AC}           \\
 $\epsilon$-Fe$_{3}$N $          $       &  $               $      &  \verb~P312~     &        11$\bar{3}$  &    76.50  &        1.2442  &            6  &          140.7  &  \cite{Jack:1952_AC}           \\
 $\alpha$-Fe$_{16}$N$_{2}        $     &  $               $      &  \verb~I4/mmm~   &         224  &    76.71  &        1.2414  &            8  &          108.2  &  \cite{Sawada:1994_PRB}        \\
 $\epsilon$-Fe                         &  Mg $            $      &  \verb~P63/mmc~  &         110  &    77.36  &        1.2325  &            6  &          116.9  &  \cite{Clendenen:1964_JPCS}    \\
 $\alpha$-FeN$_{0.0950}        $       &  $\alpha$-FeN$_{x} $    &  \verb~I4/mmm~   &         112  &    77.84  &        1.2261  &            8  &          127.7  &  \cite{Jack:1951_PRSLA}        \\
 Fe$_{3}$C$                    $       &  Fe$_{3}$C$        $    &  \verb~Pnma~     &         401  &    77.89  &        1.2255  &            4  &          145.1  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{3}$C$                    $       &  Fe$_{3}$C$        $    &  \verb~Pnma~     &         133  &    78.58  &        1.2165  &            8  &          191.3  &  \cite{Fruchart:1984_JSSC}     \\
 $\gamma$-Fe                           &  Cu$             $      &  \verb~Fm-3m~    &         220  &    78.87  &        1.2127  &           12  &          207.0  &  \cite{Haglund:1993_PRB}       \\
 $\alpha$-Fe                           &  W $             $      &  \verb~Im-3m~    &         211  &    80.13  &        1.1968  &           24  &          222.6  &  \cite{Basinski:1955_PRSLA}    \\
 Fe$_{0.7}$Ga$_{0.3}$                &  Mg $            $      &  \verb~P63/mmc~  &         103  &    80.35  &        1.1939  &           12  &          130.2  &  \cite{Schubert:1960_DN}       \\
 $\epsilon$-Fe$_{3}$C $          $       &  Fe$_{3}$N$_{1+x}  $  &  \verb~P6322~    &         113  &    80.74  &        1.1892  &           12  &          126.8  &  \cite{Lv:2008_CMS}            \\
 Fe$_{3}$Ga $                  $       &  $BiF_{3}        $    &  \verb~Fm-3m~    &         422  &    81.06  &        1.1853  &           24  &          228.2  &  \cite{Nishino:1991_SMM}       \\
 $\alpha$-Fe$_{16}$N$_{2}        $     &  $               $      &  \verb~I4/mmm~   &         422  &    81.10  &        1.1848  &           16  &          198.0  &  \cite{Sawada:1994_PRB}        \\
 $\alpha$-Fe                           &  W $             $      &  \verb~Im-3m~    &         211  &    81.65  &        1.1782  &           24  &          220.5  &  \cite{Swanson:1955_NBS}       \\
 $\alpha$-FeN$_{0.0950}        $       &  $\alpha$-FeN$_{x} $    &  \verb~I4/mmm~   &         211  &    81.65  &        1.1783  &           16  &          203.0  &  \cite{Jack:1951_PRSLA}        \\
 $\epsilon$-Fe$_{3}N_{1.39}    $     &  Mn$_{2}$N$_{1-x}  $  &  \verb~P6322~    &         302  &    82.25  &        1.1712  &           12  &          140.6  &  \cite{Leineweber:2001_JAC}    \\
 $\epsilon$-Fe$_{2.3}$N $        $       &  NiAs $          $      &  \verb~P63/mmc~  &         112  &    82.33  &        1.1702  &           12  &          110.8  &  \cite{Kim:994_JJAP}           \\
 $\alpha$-Fe                           &  W $             $      &  \verb~Im-3m~    &         211  &    82.34  &        1.1701  &           24  &          219.7  &  \cite{Straumanis:1969_ZM}     \\
 Fe$_{3}$C$                    $       &  Fe$_{3}$C$        $    &  \verb~Pnma~     &         332  &    83.02  &        1.1622  &            8  &          200.4  &  \cite{Fruchart:1984_JSSC}     \\
 $\epsilon$-Fe$_{3}$N $          $       &  Fe$_{3}$N$_{1+x}  $  &  \verb~P6322~    &         302  &    83.23  &        1.1599  &           12  &          140.6  &  \cite{Jacobs:1995_JAC}        \\
 $\epsilon$-Fe$_{3}N_{1.39}    $     &  Mn$_{2}$N$_{1-x}  $  &  \verb~P6322~    &         221  &    83.68  &        1.1548  &           12  &          118.8  &  \cite{Leineweber:2001_JAC}    \\
 Fe$_{3}$C$                    $       &  Fe$_{3}$C$        $    &  \verb~Pnma~     &         251  &    83.91  &        1.1522  &            8  &          110.2  &  \cite{Fruchart:1984_JSSC}     \\
 $\gamma^{\prime}$-GaFe$_{3}$N            &  CaTiO$_{3}      $    &  \verb~Pm-3m~    &         311  &    84.56  &        1.1450  &           24  &          244.3  &  \cite{Houben:2009_CM}         \\
 $\gamma^{\prime}$-Fe$_{4}$N $        $     &  CaTiO$_{3}      $    &  \verb~Pm-3m~    &         311  &    84.76  &        1.1427  &           24  &          266.4  &  \cite{Jacobs:1995_JAC}        \\
 $\epsilon$-Fe                         &  Mg $            $      &  \verb~P63/mmc~  &         103  &    84.92  &        1.1410  &           12  &          128.1  &  \cite{Clendenen:1964_JPCS}    \\
 $\epsilon$-Fe$_{3}$N $          $       &  Fe$_{3}$N$_{1+x}  $  &  \verb~P6322~    &         221  &    84.99  &        1.1403  &           12  &          108.2  &  \cite{Jacobs:1995_JAC}        \\
 Fe$_{3}$C$                    $       &  Fe$_{3}$C$        $    &  \verb~Pnma~     &         303  &    86.16  &        1.1278  &            4  &          123.2  &  \cite{Fruchart:1984_JSSC}     \\
 Fe$_{0.7}$Ga$_{0.3}$                &  Mg $            $      &  \verb~P63/mmc~  &         112  &    87.73  &        1.1116  &           12  &          131.6  &  \cite{Schubert:1960_DN}       \\
 Fe$_{3}$Ga $                  $       &  AuCu$_{3}       $    &  \verb~Pm-3m~    &         311  &    87.97  &        1.1093  &           24  &          236.0  &  \cite{Suzuki:1984_MTA}        \\
 Fe$_{3}$C$                    $       &  Fe$_{3}$C$        $    &  \verb~Pnma~     &         430  &    88.13  &        1.1076  &            4  &          128.8  &  \cite{Fruchart:1984_JSSC}     \\
 $\epsilon$-Fe$_{3}$C $          $       &  Fe$_{3}$N$_{1+x}  $  &  \verb~P6322~    &         302  &    88.45  &        1.1044  &           12  &          110.6  &  \cite{Lv:2008_CMS}            \\
 $\gamma$-Fe                           &  Cu$             $      &  \verb~Fm-3m~    &         311  &    88.71  &        1.1018  &           24  &          227.5  &  \cite{Straumanis:1969_ZM}     \\
 $\gamma$-FeN$_{0.0950}        $       &  $\gamma$-FeN$_{x} $    &  \verb~Fm-3m~    &         311  &    88.97  &        1.0993  &           24  &          229.3  &  \cite{Jack:1951_PRSLA}        \\
 FeGa$_{3}                   $       &  FeGa$_{3}       $    &  \verb~P42/mnm~  &         522  &    89.30  &        1.0960  &           16  &          149.5  &  \cite{Haussermann:2002_JSSC}  \\
 $\gamma$-Fe                           &  Cu$             $      &  \verb~Fm-3m~    &         311  &    90.09  &        1.0885  &           24  &          227.1  &  \cite{Westgren:1921_ZPC}      \\
 $\epsilon$-Fe                         &  Mg $            $      &  \verb~P63/mmc~  &         112  &    94.05  &        1.0528  &           12  &          128.1  &  \cite{Clendenen:1964_JPCS}    \\
 $\epsilon$-Fe$_{2.3}$N                &  NiAs $          $      &  \verb~P63/mmc~  &         202  &    94.29  &        1.0508  &           12  &          127.9  &  \cite{Kim:994_JJAP}           \\
 $\gamma$-Fe                           &  Cu$             $      &  \verb~Fm-3m~    &         311  &    96.29  &        1.0342  &           24  &          230.0  &  \cite{Haglund:1993_PRB}       \\
 $\gamma$-Fe                           &  Cu$             $      &  \verb~Fm-3m~    &         220  &    99.20  &        1.0114  &           12  &          213.9  &  \cite{Owen:1921_PM}           \\
\hline
\end{longtable}

                                    
%\bibliographystyle{apsrev4-1}
%\bibliography{/home/mauro/biblio/BIBs/library}
%Merlin.mbs v4.21 2009-07-09.
\begin{thebibliography}{10}%
\makeatletter
\providecommand \@ifxundefined [1]{%
 \ifx #1\undefined \expandafter \@firstoftwo
 \else \expandafter \@secondoftwo
\fi
}%
\providecommand \@ifnum [1]{%
 \ifnum #1\expandafter \@firstoftwo
 \else \expandafter \@secondoftwo
\fi
}%
\providecommand \enquote [1]{``#1''}%
\providecommand \bibnamefont  [1]{#1}%
\providecommand \bibfnamefont [1]{#1}%
\providecommand \citenamefont [1]{#1}%
\providecommand\href[0]{\@sanitize\@href}%
\providecommand\@href[1]{\endgroup\@@startlink{#1}\endgroup\@@href}%
\providecommand\@@href[1]{#1\@@endlink}%
\providecommand \@sanitize [0]{\begingroup\catcode`\&12\catcode`\#12\relax}%
\@ifxundefined \pdfoutput {\@firstoftwo}{%
 \@ifnum{\z@=\pdfoutput}{\@firstoftwo}{\@secondoftwo}%
}{%
 \providecommand\@@startlink[1]{\leavevmode\special{html:<a href="#1">}}%
 \providecommand\@@endlink[0]{\special{html:</a>}}%
}{%
 \providecommand\@@startlink[1]{%
  \leavevmode
  \pdfstartlink
   attr{/Border[0 0 1 ]/H/I/C[0 1 1]}%
   user{/Subtype/Link/A<</Type/Action/S/URI/URI(#1)>>}%
  \relax
 }%
 \providecommand\@@endlink[0]{\pdfendlink}%
}%
\providecommand \url  [0]{\begingroup\@sanitize \@url }%
\providecommand \@url [1]{\endgroup\@href {#1}{\urlprefix}}%
\providecommand \urlprefix [0]{URL }%
\providecommand \Eprint[0]{\href }%
\@ifxundefined \urlstyle {%
  \providecommand \doi [1]{doi:\discretionary{}{}{}#1}%
}{%
  \providecommand \doi [0]{doi:\discretionary{}{}{}\begingroup
  \urlstyle{rm}\Url }%
}%
\providecommand \doibase [0]{http://dx.doi.org/}%
\providecommand \Doi[1]{\href{\doibase#1}}%
\providecommand \bibAnnote [3]{%
  \BibitemShut{#1}%
  \begin{quotation}\noindent
    \textsc{Key:}\ #2\\\textsc{Annotation:}\ #3%
  \end{quotation}%
}%
\providecommand \bibAnnoteFile [2]{%
  \IfFileExists{#2}{\bibAnnote {#1} {#2} {\input{#2}}}{}%
}%
\providecommand \typeout [0]{\immediate \write \m@ne }%
\providecommand \selectlanguage [0]{\@gobble}%
\providecommand \bibinfo [0]{\@secondoftwo}%
\providecommand \bibfield [0]{\@secondoftwo}%
\providecommand \translation [1]{[#1]}%
\providecommand \BibitemOpen[0]{}%
\providecommand \bibitemStop [0]{}%
\providecommand \bibitemNoStop [0]{.\EOS\space}%
\providecommand \EOS [0]{\spacefactor3000\relax}%
\providecommand \BibitemShut [1]{\csname bibitem#1\endcsname}%
%</preamble>
\bibitem{Jack:1952_AC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.~H.}\ \bibnamefont{Jack}},\ }%
  \bibfield{journal}{%
  \Doi{10.1107/S0365110X52001258}{\bibinfo {journal} {Acta Crystallographica}}\
  }%
  \textbf{\bibinfo {volume} {5}},\ \bibinfo {pages} {404} (\bibinfo {month}
  {Jul.}\ \bibinfo {year} {1952}),\ ISSN \bibinfo {issn} {0365110X},\
  \url{http://scripts.iucr.org/cgi-bin/paper?S0365110X52001258}%
  \bibAnnoteFile{NoStop}{Jack:1952_AC}%
\bibitem{Pinsker:1954_DAN}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{Z.}~\bibnamefont{Pinsker}}\ and\ \bibinfo
  {author} {\bibfnamefont{S.}~\bibnamefont{Kaverin}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Doklady Akademii Nauk SSSR}\ }%
  \textbf{\bibinfo {volume} {96}},\ \bibinfo {pages} {519} (\bibinfo {year}
  {1954})%
  \bibAnnoteFile{NoStop}{Pinsker:1954_DAN}%
\bibitem{Fleet:1981_ACB}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{M.~E.}\ \bibnamefont{Fleet}},\ }%
  \bibfield{journal}{%
  \Doi{10.1107/S0567740881004597}{\bibinfo {journal} {Acta Crystallographica
  Section B Structural Crystallography and Crystal Chemistry}}\ }%
  \textbf{\bibinfo {volume} {37}},\ \bibinfo {pages} {917} (\bibinfo {month}
  {Apr.}\ \bibinfo {year} {1981}),\ ISSN \bibinfo {issn} {05677408},\
  \url{http://scripts.iucr.org/cgi-bin/paper?S0567740881004597}%
  \bibAnnoteFile{NoStop}{Fleet:1981_ACB}%
\bibitem{Haussermann:2002_JSSC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{U.}~\bibnamefont{Haussermann}},\ }%
  \bibfield{journal}{%
  \Doi{10.1006/jssc.2001.9503}{\bibinfo {journal} {Journal of Solid State
  Chemistry}}\ }%
  \textbf{\bibinfo {volume} {165}},\ \bibinfo {pages} {94} (\bibinfo {month}
  {Apr.}\ \bibinfo {year} {2002}),\ ISSN \bibinfo {issn} {00224596},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0022459601995039}%
  \bibAnnoteFile{NoStop}{Haussermann:2002_JSSC}%
\bibitem{Blake:1966_AM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{R.}~\bibnamefont{Blake}}, \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{Hessevick}}, \bibinfo {author}
  {\bibfnamefont{T.}~\bibnamefont{Zoltai}},\ and\ \bibinfo {author}
  {\bibfnamefont{L.}~\bibnamefont{Finger}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {The American Mineralogist}\ }%
  \textbf{\bibinfo {volume} {51}},\ \bibinfo {pages} {123} (\bibinfo {year}
  {1966})%
  \bibAnnoteFile{NoStop}{Blake:1966_AM}%
\bibitem{Paszkowicz:2004_JAC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{W.}~\bibnamefont{PASZKOWICZ}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/j.jallcom.2004.05.036}{\bibinfo {journal} {Journal of Alloys and
  Compounds}}\ }%
  \textbf{\bibinfo {volume} {382}},\ \bibinfo {pages} {100} (\bibinfo {month}
  {Nov.}\ \bibinfo {year} {2004}),\ ISSN \bibinfo {issn} {09258388},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0925838804007339}%
  \bibAnnoteFile{NoStop}{Paszkowicz:2004_JAC}%
\bibitem{Hasegawa:2005_JAC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{M.}~\bibnamefont{HASEGAWA}}\ and\ \bibinfo
  {author} {\bibfnamefont{T.}~\bibnamefont{YAGI}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/j.jallcom.2005.04.197}{\bibinfo {journal} {Journal of Alloys and
  Compounds}}\ }%
  \textbf{\bibinfo {volume} {403}},\ \bibinfo {pages} {131} (\bibinfo {month}
  {Nov.}\ \bibinfo {year} {2005}),\ ISSN \bibinfo {issn} {09258388},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0925838805010376}%
  \bibAnnoteFile{NoStop}{Hasegawa:2005_JAC}%
\bibitem{Leineweber:2001_JAC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{A.}~\bibnamefont{Leineweber}}, \bibinfo
  {author} {\bibfnamefont{H.}~\bibnamefont{Jacobs}}, \bibinfo {author}
  {\bibfnamefont{F.}~\bibnamefont{H\"{u}ning}}, \bibinfo {author}
  {\bibfnamefont{H.}~\bibnamefont{Lueken}},\ and\ \bibinfo {author}
  {\bibfnamefont{W.}~\bibnamefont{Kockelmann}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/S0925-8388(00)01435-3}{\bibinfo {journal} {Journal of Alloys and
  Compounds}}\ }%
  \textbf{\bibinfo {volume} {316}},\ \bibinfo {pages} {21} (\bibinfo {month}
  {Mar.}\ \bibinfo {year} {2001}),\ ISSN \bibinfo {issn} {09258388},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0925838800014353}%
  \bibAnnoteFile{NoStop}{Leineweber:2001_JAC}%
\bibitem{Kim:994_JJAP}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.-J.}\ \bibnamefont{Kim}}, \bibinfo
  {author} {\bibfnamefont{K.}~\bibnamefont{Sumiyama}}, \bibinfo {author}
  {\bibfnamefont{H.}~\bibnamefont{Onodera}},\ and\ \bibinfo {author}
  {\bibfnamefont{K.}~\bibnamefont{Suzuki}},\ }%
  \bibfield{journal}{%
  \Doi{10.1143/JJAP.33.6539}{\bibinfo {journal} {Japanese Journal of Applied
  Physics}}\ }%
  \textbf{\bibinfo {volume} {33}},\ \bibinfo {pages} {6539} (\bibinfo {month}
  {Dec.}\ \bibinfo {year} {1994}),\ ISSN \bibinfo {issn} {00214922},\
  \url{http://jjap.ipap.jp/link?JJAP/33/6539/}%
  \bibAnnoteFile{NoStop}{Kim:994_JJAP}%
\bibitem{Fruchart:1984_JSSC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{D.}~\bibnamefont{FRUCHART}}, \bibinfo
  {author} {\bibfnamefont{P.}~\bibnamefont{CHAUDOUET}}, \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{FRUCHART}}, \bibinfo {author}
  {\bibfnamefont{A.}~\bibnamefont{ROUAULT}},\ and\ \bibinfo {author}
  {\bibfnamefont{J.}~\bibnamefont{SENATEUR}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0022-4596(84)90340-2}{\bibinfo {journal} {Journal of Solid State
  Chemistry}}\ }%
  \textbf{\bibinfo {volume} {51}},\ \bibinfo {pages} {246} (\bibinfo {month}
  {Feb.}\ \bibinfo {year} {1984}),\ ISSN \bibinfo {issn} {00224596},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0022459684903402}%
  \bibAnnoteFile{NoStop}{Fruchart:1984_JSSC}%
\bibitem{Jacobs:1995_JAC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{H.}~\bibnamefont{Jacobs}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0925-8388(95)01610-4}{\bibinfo {journal} {Journal of Alloys and
  Compounds}}\ }%
  \textbf{\bibinfo {volume} {227}},\ \bibinfo {pages} {10} (\bibinfo {year}
  {1995}),\ ISSN \bibinfo {issn} {09258388},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0925838895016104}%
  \bibAnnoteFile{NoStop}{Jacobs:1995_JAC}%
\bibitem{Schubert:1960_DN}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.}~\bibnamefont{Schubert}}, \bibinfo
  {author} {\bibfnamefont{S.}~\bibnamefont{Bhan}}, \bibinfo {author}
  {\bibfnamefont{W.}~\bibnamefont{Burkhardt}}, \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{Gohle}}, \bibinfo {author}
  {\bibfnamefont{H.~G.}\ \bibnamefont{Meissner}}, \bibinfo {author}
  {\bibfnamefont{M.}~\bibnamefont{P�tzschke}},\ and\ \bibinfo {author}
  {\bibfnamefont{E.}~\bibnamefont{Stolz}},\ }%
  \bibfield{journal}{%
  \Doi{10.1007/BF00600960}{\bibinfo {journal} {Die Naturwissenschaften}}\ }%
  \textbf{\bibinfo {volume} {47}},\ \bibinfo {pages} {303} (\bibinfo {year}
  {1960}),\ ISSN \bibinfo {issn} {0028-1042},\
  \url{http://www.springerlink.com/index/10.1007/BF00600960}%
  \bibAnnoteFile{NoStop}{Schubert:1960_DN}%
\bibitem{Lv:2008_CMS}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{Z.}~\bibnamefont{LV}}, \bibinfo {author}
  {\bibfnamefont{F.}~\bibnamefont{ZHANG}}, \bibinfo {author}
  {\bibfnamefont{S.}~\bibnamefont{SUN}}, \bibinfo {author}
  {\bibfnamefont{Z.}~\bibnamefont{WANG}}, \bibinfo {author}
  {\bibfnamefont{P.}~\bibnamefont{JIANG}}, \bibinfo {author}
  {\bibfnamefont{W.}~\bibnamefont{ZHANG}},\ and\ \bibinfo {author}
  {\bibfnamefont{W.}~\bibnamefont{FU}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/j.commatsci.2008.05.006}{\bibinfo {journal} {Computational
  Materials Science}}\ }%
  \textbf{\bibinfo {volume} {44}},\ \bibinfo {pages} {690} (\bibinfo {month}
  {Dec.}\ \bibinfo {year} {2008}),\ ISSN \bibinfo {issn} {09270256},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0927025608002449}%
  \bibAnnoteFile{NoStop}{Lv:2008_CMS}%
\bibitem{Houben:2009_CM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{A.}~\bibnamefont{Houben}}, \bibinfo {author}
  {\bibfnamefont{J.}~\bibnamefont{Burghaus}},\ and\ \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{Dronskowski}},\ }%
  \bibfield{journal}{%
  \Doi{10.1021/cm901864z}{\bibinfo {journal} {Chemistry of Materials}}\ }%
  \textbf{\bibinfo {volume} {21}},\ \bibinfo {pages} {4332} (\bibinfo {month}
  {Sep.}\ \bibinfo {year} {2009}),\ ISSN \bibinfo {issn} {0897-4756},\
  \url{http://pubs.acs.org/doi/abs/10.1021/cm901864z}%
  \bibAnnoteFile{NoStop}{Houben:2009_CM}%
\bibitem{Graham:1960_JPCS}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{J.}~\bibnamefont{GRAHAM}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0022-3697(60)90170-0}{\bibinfo {journal} {Journal of Physics and
  Chemistry of Solids}}\ }%
  \textbf{\bibinfo {volume} {17}},\ \bibinfo {pages} {18} (\bibinfo {month}
  {Dec.}\ \bibinfo {year} {1960}),\ ISSN \bibinfo {issn} {00223697},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0022369760901700}%
  \bibAnnoteFile{NoStop}{Graham:1960_JPCS}%
\bibitem{Clendenen:1964_JPCS}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{R.}~\bibnamefont{CLENDENEN}}\ and\ \bibinfo
  {author} {\bibfnamefont{H.}~\bibnamefont{DRICKAMER}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0022-3697(64)90098-8}{\bibinfo {journal} {Journal of Physics and
  Chemistry of Solids}}\ }%
  \textbf{\bibinfo {volume} {25}},\ \bibinfo {pages} {865} (\bibinfo {month}
  {Aug.}\ \bibinfo {year} {1964}),\ ISSN \bibinfo {issn} {00223697},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0022369764900988}%
  \bibAnnoteFile{NoStop}{Clendenen:1964_JPCS}%
\bibitem{Suzuki:1984_MTA}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{T.}~\bibnamefont{Suzuki}}, \bibinfo {author}
  {\bibfnamefont{Y.}~\bibnamefont{Oya}},\ and\ \bibinfo {author}
  {\bibfnamefont{S.}~\bibnamefont{Ochiai}},\ }%
  \bibfield{journal}{%
  \Doi{10.1007/BF02644399}{\bibinfo {journal} {Metallurgical Transactions A}}\
  }%
  \textbf{\bibinfo {volume} {15}},\ \bibinfo {pages} {173} (\bibinfo {month}
  {Jan.}\ \bibinfo {year} {1984}),\ ISSN \bibinfo {issn} {0360-2133},\
  \url{http://www.springerlink.com/index/10.1007/BF02644399}%
  \bibAnnoteFile{NoStop}{Suzuki:1984_MTA}%
\bibitem{Sawada:1994_PRB}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{H.}~\bibnamefont{Sawada}}, \bibinfo {author}
  {\bibfnamefont{A.}~\bibnamefont{Nogami}}, \bibinfo {author}
  {\bibfnamefont{T.}~\bibnamefont{Matsumiya}},\ and\ \bibinfo {author}
  {\bibfnamefont{T.}~\bibnamefont{Oguchi}},\ }%
  \bibfield{journal}{%
  \Doi{10.1103/PhysRevB.50.10004}{\bibinfo {journal} {Physical Review B}}\ }%
  \textbf{\bibinfo {volume} {50}},\ \bibinfo {pages} {10004} (\bibinfo {month}
  {Oct.}\ \bibinfo {year} {1994}),\ ISSN \bibinfo {issn} {0163-1829},\
  \url{http://link.aps.org/doi/10.1103/PhysRevB.50.10004}%
  \bibAnnoteFile{NoStop}{Sawada:1994_PRB}%
\bibitem{Straumanis:1969_ZM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{M.}~\bibnamefont{Straumanis}}\ and\ \bibinfo
  {author} {\bibfnamefont{D.}~\bibnamefont{Kim}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Zeitschrift fuer Metallkunde}\ }%
  \textbf{\bibinfo {volume} {60}},\ \bibinfo {pages} {272} (\bibinfo {year}
  {1969})%
  \bibAnnoteFile{NoStop}{Straumanis:1969_ZM}%
\bibitem{Jack:1951_PRSLA}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.~H.}\ \bibnamefont{Jack}},\ }%
  \bibfield{journal}{%
  \Doi{10.1098/rspa.1951.0154}{\bibinfo {journal} {Proceedings of the Royal
  Society A: Mathematical, Physical and Engineering Sciences}}\ }%
  \textbf{\bibinfo {volume} {208}},\ \bibinfo {pages} {200} (\bibinfo {month}
  {Aug.}\ \bibinfo {year} {1951}),\ ISSN \bibinfo {issn} {1364-5021},\
  \url{http://rspa.royalsocietypublishing.org/cgi/doi/10.1098/rspa.1951.0154}%
  \bibAnnoteFile{NoStop}{Jack:1951_PRSLA}%
\bibitem{Westgren:1921_ZPC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{A.}~\bibnamefont{Westgren}}\ and\ \bibinfo
  {author} {\bibfnamefont{A.}~\bibnamefont{Lindh}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Zeitschrift fuer Physikalische Chemie}\ }%
  \textbf{\bibinfo {volume} {98}},\ \bibinfo {pages} {181} (\bibinfo {year}
  {1921})%
  \bibAnnoteFile{NoStop}{Westgren:1921_ZPC}%
\bibitem{Basinski:1955_PRSLA}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{Z.~S.}\ \bibnamefont{Basinski}}, \bibinfo
  {author} {\bibfnamefont{W.}~\bibnamefont{Hume-Rothery}},\ and\ \bibinfo
  {author} {\bibfnamefont{A.~L.}\ \bibnamefont{Sutton}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Proc. Royal Soc. London, A: Math. Phys. Sci.}\ }%
  \textbf{\bibinfo {volume} {229}},\ \bibinfo {pages} {459} (\bibinfo {year}
  {1955})%
  \bibAnnoteFile{NoStop}{Basinski:1955_PRSLA}%
\bibitem{Buschow:1983_JMMM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.}~\bibnamefont{BUSCHOW}}, \bibinfo
  {author} {\bibfnamefont{P.}~\bibnamefont{VANENGEN}},\ and\ \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{JONGEBREUR}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0304-8853(83)90097-5}{\bibinfo {journal} {Journal of Magnetism
  and Magnetic Materials}}\ }%
  \textbf{\bibinfo {volume} {38}},\ \bibinfo {pages} {1} (\bibinfo {month}
  {Aug.}\ \bibinfo {year} {1983}),\ ISSN \bibinfo {issn} {03048853},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0304885383900975}%
  \bibAnnoteFile{NoStop}{Buschow:1983_JMMM}%
\bibitem{Nishino:1991_SMM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{Y.}~\bibnamefont{NISHINO}}, \bibinfo
  {author} {\bibfnamefont{M.}~\bibnamefont{MATSUO}}, \bibinfo {author}
  {\bibfnamefont{S.}~\bibnamefont{ASANO}},\ and\ \bibinfo {author}
  {\bibfnamefont{N.}~\bibnamefont{KAWAMIYA}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0956-716X(91)90017-U}{\bibinfo {journal} {Scripta Metallurgica
  et Materialia}}\ }%
  \textbf{\bibinfo {volume} {25}},\ \bibinfo {pages} {2291} (\bibinfo {month}
  {Oct.}\ \bibinfo {year} {1991}),\ ISSN \bibinfo {issn} {0956716X},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0956716X9190017U}%
  \bibAnnoteFile{NoStop}{Nishino:1991_SMM}%
\bibitem{Swanson:1955_NBS}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{H.~E.}\ \bibnamefont{Swanson}}\ and\
  \bibinfo {author} {\bibfnamefont{E.}~\bibnamefont{Tatge}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {National Bureau of Standards}\ }%
  \textbf{\bibinfo {volume} {539}},\ \bibinfo {pages} {1} (\bibinfo {year}
  {1955})%
  \bibAnnoteFile{NoStop}{Swanson:1955_NBS}%
\bibitem{Haglund:1993_PRB}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{J.}~\bibnamefont{H\"{a}glund}}, \bibinfo
  {author} {\bibfnamefont{A.}~\bibnamefont{{Fern\'{a}ndez Guillermet}}},
  \bibinfo {author} {\bibfnamefont{G.}~\bibnamefont{Grimvall}},\ and\ \bibinfo
  {author} {\bibfnamefont{M.}~\bibnamefont{K\"{o}rling}},\ }%
  \bibfield{journal}{%
  \Doi{10.1103/PhysRevB.48.11685}{\bibinfo {journal} {Physical Review B}}\ }%
  \textbf{\bibinfo {volume} {48}},\ \bibinfo {pages} {11685} (\bibinfo {month}
  {Oct.}\ \bibinfo {year} {1993}),\ ISSN \bibinfo {issn} {0163-1829},\
  \url{http://link.aps.org/doi/10.1103/PhysRevB.48.11685}%
  \bibAnnoteFile{NoStop}{Haglund:1993_PRB}%
\bibitem{Owen:1921_PM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{E.}~\bibnamefont{Owen}}\ and\ \bibinfo
  {author} {\bibfnamefont{E.}~\bibnamefont{Yates}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Philosophical Magazine}\ }%
  \textbf{\bibinfo {volume} {15}},\ \bibinfo {pages} {472} (\bibinfo {year}
  {1921})%
  \bibAnnoteFile{NoStop}{Owen:1921_PM}%
\end{thebibliography}%

\end{document}

1208.3420.extracted_bib
\begin{thebibliography}{10}%
\makeatletter
\providecommand \@ifxundefined [1]{%
 \ifx #1\undefined \expandafter \@firstoftwo
 \else \expandafter \@secondoftwo
\fi
}%
\providecommand \@ifnum [1]{%
 \ifnum #1\expandafter \@firstoftwo
 \else \expandafter \@secondoftwo
\fi
}%
\providecommand \enquote [1]{``#1''}%
\providecommand \bibnamefont  [1]{#1}%
\providecommand \bibfnamefont [1]{#1}%
\providecommand \citenamefont [1]{#1}%
\providecommand\href[0]{\@sanitize\@href}%
\providecommand\@href[1]{\endgroup\@@startlink{#1}\endgroup\@@href}%
\providecommand\@@href[1]{#1\@@endlink}%
\providecommand \@sanitize [0]{\begingroup\catcode`\&12\catcode`\#12\relax}%
\@ifxundefined \pdfoutput {\@firstoftwo}{%
 \@ifnum{\z@=\pdfoutput}{\@firstoftwo}{\@secondoftwo}%
}{%
 \providecommand\@@startlink[1]{\leavevmode\special{html:<a href="#1">}}%
 \providecommand\@@endlink[0]{\special{html:</a>}}%
}{%
 \providecommand\@@startlink[1]{%
  \leavevmode
  \pdfstartlink
   attr{/Border[0 0 1 ]/H/I/C[0 1 1]}%
   user{/Subtype/Link/A<</Type/Action/S/URI/URI(#1)>>}%
  \relax
 }%
 \providecommand\@@endlink[0]{\pdfendlink}%
}%
\providecommand \url  [0]{\begingroup\@sanitize \@url }%
\providecommand \@url [1]{\endgroup\@href {#1}{\urlprefix}}%
\providecommand \urlprefix [0]{URL }%
\providecommand \Eprint[0]{\href }%
\@ifxundefined \urlstyle {%
  \providecommand \doi [1]{doi:\discretionary{}{}{}#1}%
}{%
  \providecommand \doi [0]{doi:\discretionary{}{}{}\begingroup
  \urlstyle{rm}\Url }%
}%
\providecommand \doibase [0]{http://dx.doi.org/}%
\providecommand \Doi[1]{\href{\doibase#1}}%
\providecommand \bibAnnote [3]{%
  \BibitemShut{#1}%
  \begin{quotation}\noindent
    \textsc{Key:}\ #2\\\textsc{Annotation:}\ #3%
  \end{quotation}%
}%
\providecommand \bibAnnoteFile [2]{%
  \IfFileExists{#2}{\bibAnnote {#1} {#2} {\input{#2}}}{}%
}%
\providecommand \typeout [0]{\immediate \write \m@ne }%
\providecommand \selectlanguage [0]{\@gobble}%
\providecommand \bibinfo [0]{\@secondoftwo}%
\providecommand \bibfield [0]{\@secondoftwo}%
\providecommand \translation [1]{[#1]}%
\providecommand \BibitemOpen[0]{}%
\providecommand \bibitemStop [0]{}%
\providecommand \bibitemNoStop [0]{.\EOS\space}%
\providecommand \EOS [0]{\spacefactor3000\relax}%
\providecommand \BibitemShut [1]{\csname bibitem#1\endcsname}%
%</preamble>
\bibitem{Jack:1952_AC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.~H.}\ \bibnamefont{Jack}},\ }%
  \bibfield{journal}{%
  \Doi{10.1107/S0365110X52001258}{\bibinfo {journal} {Acta Crystallographica}}\
  }%
  \textbf{\bibinfo {volume} {5}},\ \bibinfo {pages} {404} (\bibinfo {month}
  {Jul.}\ \bibinfo {year} {1952}),\ ISSN \bibinfo {issn} {0365110X},\
  \url{http://scripts.iucr.org/cgi-bin/paper?S0365110X52001258}%
  \bibAnnoteFile{NoStop}{Jack:1952_AC}%
\bibitem{Pinsker:1954_DAN}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{Z.}~\bibnamefont{Pinsker}}\ and\ \bibinfo
  {author} {\bibfnamefont{S.}~\bibnamefont{Kaverin}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Doklady Akademii Nauk SSSR}\ }%
  \textbf{\bibinfo {volume} {96}},\ \bibinfo {pages} {519} (\bibinfo {year}
  {1954})%
  \bibAnnoteFile{NoStop}{Pinsker:1954_DAN}%
\bibitem{Fleet:1981_ACB}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{M.~E.}\ \bibnamefont{Fleet}},\ }%
  \bibfield{journal}{%
  \Doi{10.1107/S0567740881004597}{\bibinfo {journal} {Acta Crystallographica
  Section B Structural Crystallography and Crystal Chemistry}}\ }%
  \textbf{\bibinfo {volume} {37}},\ \bibinfo {pages} {917} (\bibinfo {month}
  {Apr.}\ \bibinfo {year} {1981}),\ ISSN \bibinfo {issn} {05677408},\
  \url{http://scripts.iucr.org/cgi-bin/paper?S0567740881004597}%
  \bibAnnoteFile{NoStop}{Fleet:1981_ACB}%
\bibitem{Haussermann:2002_JSSC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{U.}~\bibnamefont{Haussermann}},\ }%
  \bibfield{journal}{%
  \Doi{10.1006/jssc.2001.9503}{\bibinfo {journal} {Journal of Solid State
  Chemistry}}\ }%
  \textbf{\bibinfo {volume} {165}},\ \bibinfo {pages} {94} (\bibinfo {month}
  {Apr.}\ \bibinfo {year} {2002}),\ ISSN \bibinfo {issn} {00224596},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0022459601995039}%
  \bibAnnoteFile{NoStop}{Haussermann:2002_JSSC}%
\bibitem{Blake:1966_AM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{R.}~\bibnamefont{Blake}}, \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{Hessevick}}, \bibinfo {author}
  {\bibfnamefont{T.}~\bibnamefont{Zoltai}},\ and\ \bibinfo {author}
  {\bibfnamefont{L.}~\bibnamefont{Finger}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {The American Mineralogist}\ }%
  \textbf{\bibinfo {volume} {51}},\ \bibinfo {pages} {123} (\bibinfo {year}
  {1966})%
  \bibAnnoteFile{NoStop}{Blake:1966_AM}%
\bibitem{Paszkowicz:2004_JAC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{W.}~\bibnamefont{PASZKOWICZ}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/j.jallcom.2004.05.036}{\bibinfo {journal} {Journal of Alloys and
  Compounds}}\ }%
  \textbf{\bibinfo {volume} {382}},\ \bibinfo {pages} {100} (\bibinfo {month}
  {Nov.}\ \bibinfo {year} {2004}),\ ISSN \bibinfo {issn} {09258388},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0925838804007339}%
  \bibAnnoteFile{NoStop}{Paszkowicz:2004_JAC}%
\bibitem{Hasegawa:2005_JAC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{M.}~\bibnamefont{HASEGAWA}}\ and\ \bibinfo
  {author} {\bibfnamefont{T.}~\bibnamefont{YAGI}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/j.jallcom.2005.04.197}{\bibinfo {journal} {Journal of Alloys and
  Compounds}}\ }%
  \textbf{\bibinfo {volume} {403}},\ \bibinfo {pages} {131} (\bibinfo {month}
  {Nov.}\ \bibinfo {year} {2005}),\ ISSN \bibinfo {issn} {09258388},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0925838805010376}%
  \bibAnnoteFile{NoStop}{Hasegawa:2005_JAC}%
\bibitem{Leineweber:2001_JAC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{A.}~\bibnamefont{Leineweber}}, \bibinfo
  {author} {\bibfnamefont{H.}~\bibnamefont{Jacobs}}, \bibinfo {author}
  {\bibfnamefont{F.}~\bibnamefont{H\"{u}ning}}, \bibinfo {author}
  {\bibfnamefont{H.}~\bibnamefont{Lueken}},\ and\ \bibinfo {author}
  {\bibfnamefont{W.}~\bibnamefont{Kockelmann}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/S0925-8388(00)01435-3}{\bibinfo {journal} {Journal of Alloys and
  Compounds}}\ }%
  \textbf{\bibinfo {volume} {316}},\ \bibinfo {pages} {21} (\bibinfo {month}
  {Mar.}\ \bibinfo {year} {2001}),\ ISSN \bibinfo {issn} {09258388},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0925838800014353}%
  \bibAnnoteFile{NoStop}{Leineweber:2001_JAC}%
\bibitem{Kim:994_JJAP}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.-J.}\ \bibnamefont{Kim}}, \bibinfo
  {author} {\bibfnamefont{K.}~\bibnamefont{Sumiyama}}, \bibinfo {author}
  {\bibfnamefont{H.}~\bibnamefont{Onodera}},\ and\ \bibinfo {author}
  {\bibfnamefont{K.}~\bibnamefont{Suzuki}},\ }%
  \bibfield{journal}{%
  \Doi{10.1143/JJAP.33.6539}{\bibinfo {journal} {Japanese Journal of Applied
  Physics}}\ }%
  \textbf{\bibinfo {volume} {33}},\ \bibinfo {pages} {6539} (\bibinfo {month}
  {Dec.}\ \bibinfo {year} {1994}),\ ISSN \bibinfo {issn} {00214922},\
  \url{http://jjap.ipap.jp/link?JJAP/33/6539/}%
  \bibAnnoteFile{NoStop}{Kim:994_JJAP}%
\bibitem{Fruchart:1984_JSSC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{D.}~\bibnamefont{FRUCHART}}, \bibinfo
  {author} {\bibfnamefont{P.}~\bibnamefont{CHAUDOUET}}, \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{FRUCHART}}, \bibinfo {author}
  {\bibfnamefont{A.}~\bibnamefont{ROUAULT}},\ and\ \bibinfo {author}
  {\bibfnamefont{J.}~\bibnamefont{SENATEUR}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0022-4596(84)90340-2}{\bibinfo {journal} {Journal of Solid State
  Chemistry}}\ }%
  \textbf{\bibinfo {volume} {51}},\ \bibinfo {pages} {246} (\bibinfo {month}
  {Feb.}\ \bibinfo {year} {1984}),\ ISSN \bibinfo {issn} {00224596},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0022459684903402}%
  \bibAnnoteFile{NoStop}{Fruchart:1984_JSSC}%
\bibitem{Jacobs:1995_JAC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{H.}~\bibnamefont{Jacobs}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0925-8388(95)01610-4}{\bibinfo {journal} {Journal of Alloys and
  Compounds}}\ }%
  \textbf{\bibinfo {volume} {227}},\ \bibinfo {pages} {10} (\bibinfo {year}
  {1995}),\ ISSN \bibinfo {issn} {09258388},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0925838895016104}%
  \bibAnnoteFile{NoStop}{Jacobs:1995_JAC}%
\bibitem{Schubert:1960_DN}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.}~\bibnamefont{Schubert}}, \bibinfo
  {author} {\bibfnamefont{S.}~\bibnamefont{Bhan}}, \bibinfo {author}
  {\bibfnamefont{W.}~\bibnamefont{Burkhardt}}, \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{Gohle}}, \bibinfo {author}
  {\bibfnamefont{H.~G.}\ \bibnamefont{Meissner}}, \bibinfo {author}
  {\bibfnamefont{M.}~\bibnamefont{P�tzschke}},\ and\ \bibinfo {author}
  {\bibfnamefont{E.}~\bibnamefont{Stolz}},\ }%
  \bibfield{journal}{%
  \Doi{10.1007/BF00600960}{\bibinfo {journal} {Die Naturwissenschaften}}\ }%
  \textbf{\bibinfo {volume} {47}},\ \bibinfo {pages} {303} (\bibinfo {year}
  {1960}),\ ISSN \bibinfo {issn} {0028-1042},\
  \url{http://www.springerlink.com/index/10.1007/BF00600960}%
  \bibAnnoteFile{NoStop}{Schubert:1960_DN}%
\bibitem{Lv:2008_CMS}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{Z.}~\bibnamefont{LV}}, \bibinfo {author}
  {\bibfnamefont{F.}~\bibnamefont{ZHANG}}, \bibinfo {author}
  {\bibfnamefont{S.}~\bibnamefont{SUN}}, \bibinfo {author}
  {\bibfnamefont{Z.}~\bibnamefont{WANG}}, \bibinfo {author}
  {\bibfnamefont{P.}~\bibnamefont{JIANG}}, \bibinfo {author}
  {\bibfnamefont{W.}~\bibnamefont{ZHANG}},\ and\ \bibinfo {author}
  {\bibfnamefont{W.}~\bibnamefont{FU}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/j.commatsci.2008.05.006}{\bibinfo {journal} {Computational
  Materials Science}}\ }%
  \textbf{\bibinfo {volume} {44}},\ \bibinfo {pages} {690} (\bibinfo {month}
  {Dec.}\ \bibinfo {year} {2008}),\ ISSN \bibinfo {issn} {09270256},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/S0927025608002449}%
  \bibAnnoteFile{NoStop}{Lv:2008_CMS}%
\bibitem{Houben:2009_CM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{A.}~\bibnamefont{Houben}}, \bibinfo {author}
  {\bibfnamefont{J.}~\bibnamefont{Burghaus}},\ and\ \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{Dronskowski}},\ }%
  \bibfield{journal}{%
  \Doi{10.1021/cm901864z}{\bibinfo {journal} {Chemistry of Materials}}\ }%
  \textbf{\bibinfo {volume} {21}},\ \bibinfo {pages} {4332} (\bibinfo {month}
  {Sep.}\ \bibinfo {year} {2009}),\ ISSN \bibinfo {issn} {0897-4756},\
  \url{http://pubs.acs.org/doi/abs/10.1021/cm901864z}%
  \bibAnnoteFile{NoStop}{Houben:2009_CM}%
\bibitem{Graham:1960_JPCS}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{J.}~\bibnamefont{GRAHAM}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0022-3697(60)90170-0}{\bibinfo {journal} {Journal of Physics and
  Chemistry of Solids}}\ }%
  \textbf{\bibinfo {volume} {17}},\ \bibinfo {pages} {18} (\bibinfo {month}
  {Dec.}\ \bibinfo {year} {1960}),\ ISSN \bibinfo {issn} {00223697},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0022369760901700}%
  \bibAnnoteFile{NoStop}{Graham:1960_JPCS}%
\bibitem{Clendenen:1964_JPCS}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{R.}~\bibnamefont{CLENDENEN}}\ and\ \bibinfo
  {author} {\bibfnamefont{H.}~\bibnamefont{DRICKAMER}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0022-3697(64)90098-8}{\bibinfo {journal} {Journal of Physics and
  Chemistry of Solids}}\ }%
  \textbf{\bibinfo {volume} {25}},\ \bibinfo {pages} {865} (\bibinfo {month}
  {Aug.}\ \bibinfo {year} {1964}),\ ISSN \bibinfo {issn} {00223697},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0022369764900988}%
  \bibAnnoteFile{NoStop}{Clendenen:1964_JPCS}%
\bibitem{Suzuki:1984_MTA}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{T.}~\bibnamefont{Suzuki}}, \bibinfo {author}
  {\bibfnamefont{Y.}~\bibnamefont{Oya}},\ and\ \bibinfo {author}
  {\bibfnamefont{S.}~\bibnamefont{Ochiai}},\ }%
  \bibfield{journal}{%
  \Doi{10.1007/BF02644399}{\bibinfo {journal} {Metallurgical Transactions A}}\
  }%
  \textbf{\bibinfo {volume} {15}},\ \bibinfo {pages} {173} (\bibinfo {month}
  {Jan.}\ \bibinfo {year} {1984}),\ ISSN \bibinfo {issn} {0360-2133},\
  \url{http://www.springerlink.com/index/10.1007/BF02644399}%
  \bibAnnoteFile{NoStop}{Suzuki:1984_MTA}%
\bibitem{Sawada:1994_PRB}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{H.}~\bibnamefont{Sawada}}, \bibinfo {author}
  {\bibfnamefont{A.}~\bibnamefont{Nogami}}, \bibinfo {author}
  {\bibfnamefont{T.}~\bibnamefont{Matsumiya}},\ and\ \bibinfo {author}
  {\bibfnamefont{T.}~\bibnamefont{Oguchi}},\ }%
  \bibfield{journal}{%
  \Doi{10.1103/PhysRevB.50.10004}{\bibinfo {journal} {Physical Review B}}\ }%
  \textbf{\bibinfo {volume} {50}},\ \bibinfo {pages} {10004} (\bibinfo {month}
  {Oct.}\ \bibinfo {year} {1994}),\ ISSN \bibinfo {issn} {0163-1829},\
  \url{http://link.aps.org/doi/10.1103/PhysRevB.50.10004}%
  \bibAnnoteFile{NoStop}{Sawada:1994_PRB}%
\bibitem{Straumanis:1969_ZM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{M.}~\bibnamefont{Straumanis}}\ and\ \bibinfo
  {author} {\bibfnamefont{D.}~\bibnamefont{Kim}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Zeitschrift fuer Metallkunde}\ }%
  \textbf{\bibinfo {volume} {60}},\ \bibinfo {pages} {272} (\bibinfo {year}
  {1969})%
  \bibAnnoteFile{NoStop}{Straumanis:1969_ZM}%
\bibitem{Jack:1951_PRSLA}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.~H.}\ \bibnamefont{Jack}},\ }%
  \bibfield{journal}{%
  \Doi{10.1098/rspa.1951.0154}{\bibinfo {journal} {Proceedings of the Royal
  Society A: Mathematical, Physical and Engineering Sciences}}\ }%
  \textbf{\bibinfo {volume} {208}},\ \bibinfo {pages} {200} (\bibinfo {month}
  {Aug.}\ \bibinfo {year} {1951}),\ ISSN \bibinfo {issn} {1364-5021},\
  \url{http://rspa.royalsocietypublishing.org/cgi/doi/10.1098/rspa.1951.0154}%
  \bibAnnoteFile{NoStop}{Jack:1951_PRSLA}%
\bibitem{Westgren:1921_ZPC}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{A.}~\bibnamefont{Westgren}}\ and\ \bibinfo
  {author} {\bibfnamefont{A.}~\bibnamefont{Lindh}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Zeitschrift fuer Physikalische Chemie}\ }%
  \textbf{\bibinfo {volume} {98}},\ \bibinfo {pages} {181} (\bibinfo {year}
  {1921})%
  \bibAnnoteFile{NoStop}{Westgren:1921_ZPC}%
\bibitem{Basinski:1955_PRSLA}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{Z.~S.}\ \bibnamefont{Basinski}}, \bibinfo
  {author} {\bibfnamefont{W.}~\bibnamefont{Hume-Rothery}},\ and\ \bibinfo
  {author} {\bibfnamefont{A.~L.}\ \bibnamefont{Sutton}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Proc. Royal Soc. London, A: Math. Phys. Sci.}\ }%
  \textbf{\bibinfo {volume} {229}},\ \bibinfo {pages} {459} (\bibinfo {year}
  {1955})%
  \bibAnnoteFile{NoStop}{Basinski:1955_PRSLA}%
\bibitem{Buschow:1983_JMMM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{K.}~\bibnamefont{BUSCHOW}}, \bibinfo
  {author} {\bibfnamefont{P.}~\bibnamefont{VANENGEN}},\ and\ \bibinfo {author}
  {\bibfnamefont{R.}~\bibnamefont{JONGEBREUR}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0304-8853(83)90097-5}{\bibinfo {journal} {Journal of Magnetism
  and Magnetic Materials}}\ }%
  \textbf{\bibinfo {volume} {38}},\ \bibinfo {pages} {1} (\bibinfo {month}
  {Aug.}\ \bibinfo {year} {1983}),\ ISSN \bibinfo {issn} {03048853},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0304885383900975}%
  \bibAnnoteFile{NoStop}{Buschow:1983_JMMM}%
\bibitem{Nishino:1991_SMM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{Y.}~\bibnamefont{NISHINO}}, \bibinfo
  {author} {\bibfnamefont{M.}~\bibnamefont{MATSUO}}, \bibinfo {author}
  {\bibfnamefont{S.}~\bibnamefont{ASANO}},\ and\ \bibinfo {author}
  {\bibfnamefont{N.}~\bibnamefont{KAWAMIYA}},\ }%
  \bibfield{journal}{%
  \Doi{10.1016/0956-716X(91)90017-U}{\bibinfo {journal} {Scripta Metallurgica
  et Materialia}}\ }%
  \textbf{\bibinfo {volume} {25}},\ \bibinfo {pages} {2291} (\bibinfo {month}
  {Oct.}\ \bibinfo {year} {1991}),\ ISSN \bibinfo {issn} {0956716X},\
  \url{http://linkinghub.elsevier.com/retrieve/pii/0956716X9190017U}%
  \bibAnnoteFile{NoStop}{Nishino:1991_SMM}%
\bibitem{Swanson:1955_NBS}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{H.~E.}\ \bibnamefont{Swanson}}\ and\
  \bibinfo {author} {\bibfnamefont{E.}~\bibnamefont{Tatge}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {National Bureau of Standards}\ }%
  \textbf{\bibinfo {volume} {539}},\ \bibinfo {pages} {1} (\bibinfo {year}
  {1955})%
  \bibAnnoteFile{NoStop}{Swanson:1955_NBS}%
\bibitem{Haglund:1993_PRB}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{J.}~\bibnamefont{H\"{a}glund}}, \bibinfo
  {author} {\bibfnamefont{A.}~\bibnamefont{{Fern\'{a}ndez Guillermet}}},
  \bibinfo {author} {\bibfnamefont{G.}~\bibnamefont{Grimvall}},\ and\ \bibinfo
  {author} {\bibfnamefont{M.}~\bibnamefont{K\"{o}rling}},\ }%
  \bibfield{journal}{%
  \Doi{10.1103/PhysRevB.48.11685}{\bibinfo {journal} {Physical Review B}}\ }%
  \textbf{\bibinfo {volume} {48}},\ \bibinfo {pages} {11685} (\bibinfo {month}
  {Oct.}\ \bibinfo {year} {1993}),\ ISSN \bibinfo {issn} {0163-1829},\
  \url{http://link.aps.org/doi/10.1103/PhysRevB.48.11685}%
  \bibAnnoteFile{NoStop}{Haglund:1993_PRB}%
\bibitem{Owen:1921_PM}%
  \BibitemOpen
  \bibfield{author}{%
  \bibinfo {author} {\bibfnamefont{E.}~\bibnamefont{Owen}}\ and\ \bibinfo
  {author} {\bibfnamefont{E.}~\bibnamefont{Yates}},\ }%
  \bibfield{journal}{%
  \bibinfo {journal} {Philosophical Magazine}\ }%
  \textbf{\bibinfo {volume} {15}},\ \bibinfo {pages} {472} (\bibinfo {year}
  {1921})%
  \bibAnnoteFile{NoStop}{Owen:1921_PM}%
\end{thebibliography}